#------------------------------------------------------------------------------
#$Date: 2017-10-07 05:55:02 +0300 (Sat, 07 Oct 2017) $
#$Revision: 201844 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/04/44/7044429.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7044429
loop_
_publ_author_name
'Huang, Hui-Lin'
'Liu, You-Rong'
'Huang, Li-Hsun'
'Chiang, Ray-Kuang'
'Wang, Sue-Lein'
_publ_section_title
;
 Achiral Polyamine-Induced Chiral Zinc Gallophosphates with Fused Double
 Helix-Like Strands Exhibiting Blue to Green Photoluminescence
;
_journal_name_full               'Dalton Trans.'
_journal_paper_doi               10.1039/C7DT02465G
_journal_year                    2017
_chemical_formula_sum            'C0.9 H3.3 Ga0.4 N0.6 O4 P Zn0.6'
_chemical_formula_weight         184.62
_chemical_name_common            ZG-4N-L
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      cubic
_space_group_IT_number           214
_space_group_name_Hall           'I 4bd 2c 3'
_space_group_name_H-M_alt        'I 41 3 2'
_symmetry_space_group_name_Hall  'I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I 41 3 2'
_audit_block_doi                 10.5517/ccdc.csd.cc1pd508
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2017-09-20 deposited with the CCDC.
2017-10-04 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            48
_cell_length_a                   17.9925(6)
_cell_length_b                   17.9925(6)
_cell_length_c                   17.9925(6)
_cell_measurement_reflns_used    19721
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.292
_cell_measurement_theta_min      3.201
_cell_volume                     5824.7(3)
_computing_cell_refinement       'SAINT V8.34A (Bruker AXS Inc., 2013)'
_computing_data_collection       'APEX2 (Bruker AXS, 2010)'
_computing_data_reduction        'SAINT V8.34A (Bruker AXS Inc., 2013)'
_computing_molecular_graphics    'SHELXTL (Sheldrick, 2008)'
_computing_publication_material  SHELXTL
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      296(2)
_diffrn_detector_area_resol_mean 8.3333
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0232
_diffrn_reflns_av_unetI/netI     0.0143
_diffrn_reflns_Laue_measured_fraction_full 0.991
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            28114
_diffrn_reflns_point_group_measured_fraction_full 0.994
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.295
_diffrn_reflns_theta_min         1.601
_exptl_absorpt_coefficient_mu    5.538
_exptl_absorpt_correction_T_max  0.9485
_exptl_absorpt_correction_T_min  0.8523
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS V2014/2 (Bruker AXS Inc.)'
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    2.526
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Cube
_exptl_crystal_F_000             4334
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.15
_platon_squeeze_details
;
The integral electron density in the voids is 655 electrons. The elctron density for N4C6H22 (protonated triethylenetetramine) calculated from the formula (N4C6H22)0.15(Zn0.6Ga0.4PO4) is 619 electrons.
;
_refine_diff_density_max         0.251
_refine_diff_density_min         -0.169
_refine_diff_density_rms         0.047
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.014(12)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.132
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     56
_refine_ls_number_reflns         1214
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.132
_refine_ls_R_factor_all          0.0131
_refine_ls_R_factor_gt           0.0125
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0177P)²+3.1693P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0360
_refine_ls_wR_factor_ref         0.0362
_reflns_Friedel_coverage         0.649
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     1.000
_reflns_number_gt                1191
_reflns_number_total             1214
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c7dt02465g2.cif
_cod_data_source_block           ZG-4N-L
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_original_cell_volume        5824.7(6)
_cod_original_formula_sum        'C0.90 H3.30 Ga0.40 N0.60 O4 P Zn0.60'
_cod_database_code               7044429
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelxl_version_number           2014-3
_platon_squeeze_void_probe_radius 1.20
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'z, x, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z, x'
'-y, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z, x+1/2'
'y+3/4, x+1/4, -z+1/4'
'-y+3/4, -x+3/4, -z+3/4'
'y+1/4, -x+1/4, z+3/4'
'-y+1/4, x+3/4, z+1/4'
'x+3/4, z+1/4, -y+1/4'
'-x+1/4, z+3/4, y+1/4'
'-x+3/4, -z+3/4, -y+3/4'
'x+1/4, -z+1/4, y+3/4'
'z+3/4, y+1/4, -x+1/4'
'z+1/4, -y+1/4, x+3/4'
'-z+1/4, y+3/4, x+1/4'
'-z+3/4, -y+3/4, -x+3/4'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-x+1/2, y+1, -z+1'
'x+1, -y+1, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1, -x+1, -y+1/2'
'-z+1, -x+1/2, y+1'
'-z+1/2, x+1, -y+1'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1, -x+1'
'y+1, -z+1, -x+1/2'
'-y+1, -z+1/2, x+1'
'y+5/4, x+3/4, -z+3/4'
'-y+5/4, -x+5/4, -z+5/4'
'y+3/4, -x+3/4, z+5/4'
'-y+3/4, x+5/4, z+3/4'
'x+5/4, z+3/4, -y+3/4'
'-x+3/4, z+5/4, y+3/4'
'-x+5/4, -z+5/4, -y+5/4'
'x+3/4, -z+3/4, y+5/4'
'z+5/4, y+3/4, -x+3/4'
'z+3/4, -y+3/4, x+5/4'
'-z+3/4, y+5/4, x+3/4'
'-z+5/4, -y+5/4, -x+5/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_occupancy
Ga1 Ga 0.24167(2) 0.34778(2) 0.88867(2) 0.01782(8) Uani 0.4 1 d P
Zn1 Zn 0.24167(2) 0.34778(2) 0.88867(2) 0.01782(8) Uani 0.6 1 d P
P1 P 0.34814(3) 0.38503(3) 0.75695(3) 0.01767(13) Uani 1 1 d .
O1 O 0.27483(10) 0.39158(11) 0.79981(9) 0.0281(4) Uani 1 1 d .
O2 O 0.19634(9) 0.25380(9) 0.87054(11) 0.0282(4) Uani 1 1 d .
O3 O 0.32644(9) 0.33774(10) 0.95187(10) 0.0263(4) Uani 1 1 d .
O4 O 0.17302(10) 0.41524(10) 0.93149(9) 0.0259(4) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Ga1 O4 106.51(8) . .
O1 Ga1 O2 111.24(8) . .
O4 Ga1 O2 111.04(7) . .
O1 Ga1 O3 107.00(8) . .
O4 Ga1 O3 109.81(8) . .
O2 Ga1 O3 111.07(7) . .
O2 P1 O1 111.32(10) 6_456 .
O2 P1 O3 107.15(10) 6_456 14_556
O1 P1 O3 111.64(10) . 14_556
O2 P1 O4 110.77(10) 6_456 40_544
O1 P1 O4 105.97(9) . 40_544
O3 P1 O4 110.04(10) 14_556 40_544
P1 O1 Ga1 131.99(11) . .
P1 O2 Ga1 124.51(10) 12_565 .
P1 O3 Ga1 125.17(11) 14_556 .
P1 O4 Ga1 123.21(11) 39_454 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ga1 O1 1.8796(17) .
Ga1 O4 1.8954(17) .
Ga1 O2 1.9055(16) .
Ga1 O3 1.9111(16) .
P1 O2 1.5308(17) 6_456
P1 O1 1.5325(17) .
P1 O3 1.5364(18) 14_556
P1 O4 1.5390(17) 40_544
O2 P1 1.5308(17) 12_565
O3 P1 1.5365(18) 14_556
O4 P1 1.5389(17) 39_454
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.014 0.226 0.133 939 314 ' '
2 -0.020 0.224 0.624 995 341 ' '
